#------------------------------------------------------------------------------
#$Date: 2018-07-30 13:15:24 +0300 (Mon, 30 Jul 2018) $
#$Revision: 209296 $
#$URL: file:///home/coder/svn-repositories/cod/cif/4/00/06/4000683.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4000683
loop_
_publ_author_name
'Ok, Kang Min'
'Halasyamani, P. Shiv'
_publ_section_title
;
 New Tellurites: Syntheses, Structures, and Characterization of
 K2Te4O9·3.2H2O, KGaTe6O14, and KGaTe2O6·1.8H2O
;
_journal_coden_ASTM              CMATEX
_journal_issue                   11
_journal_name_full               'Chemistry of Materials'
_journal_page_first              4278
_journal_page_last               4284
_journal_paper_doi               10.1021/cm0103489
_journal_volume                  13
_journal_year                    2001
_chemical_formula_sum            'H8 K2 O12.2 Te4'
_chemical_formula_weight         790.20
_space_group_IT_number           1
_symmetry_cell_setting           triclinic
_symmetry_Int_Tables_number      1
_symmetry_space_group_name_Hall  'P 1'
_symmetry_space_group_name_H-M   'P 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_cell_angle_alpha                60.8490(10)
_cell_angle_beta                 69.9180(10)
_cell_angle_gamma                85.9680(10)
_cell_formula_units_Z            2
_cell_length_a                   7.5046(5)
_cell_length_b                   10.7097(8)
_cell_length_c                   10.7159(8)
_cell_measurement_temperature    293.0(2)
_cell_volume                     701.49(9)
_diffrn_ambient_temperature      293.0(2)
_diffrn_measured_fraction_theta_full 0.93
_diffrn_measured_fraction_theta_max 0.93
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.035
_diffrn_reflns_av_unetI/netI     0.019
_diffrn_reflns_limit_h_max       6
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_k_max       12
_diffrn_reflns_limit_k_min       -13
_diffrn_reflns_limit_l_max       9
_diffrn_reflns_limit_l_min       -13
_diffrn_reflns_number            4283
_diffrn_reflns_theta_full        27.48
_diffrn_reflns_theta_max         27.48
_diffrn_reflns_theta_min         2.19
_exptl_absorpt_coefficient_mu    8.886
_exptl_crystal_density_diffrn    3.81
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             716
_exptl_crystal_size_max          0.05
_exptl_crystal_size_mid          0.25
_exptl_crystal_size_min          0.30
_refine_diff_density_max         1.697
_refine_diff_density_min         -1.555
_refine_diff_density_rms         0.284
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.56(4)
_refine_ls_extinction_coef       0.0040(3)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.073
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     344
_refine_ls_number_reflns         3540
_refine_ls_number_restraints     3
_refine_ls_restrained_S_all      1.072
_refine_ls_R_factor_all          0.0316
_refine_ls_R_factor_gt           0.0313
_refine_ls_shift/su_max          0.004
_refine_ls_shift/su_mean         0.001
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0671P)²+2.0015P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0856
_refine_ls_wR_factor_ref         0.0859
_reflns_number_gt                3491
_reflns_number_total             3540
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            4000094_b.cif
_cod_database_code               4000683
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Te1 Te 0.53829(10) 0.84045(7) 0.81729(7) 0.01693(19) Uani 1 1 d .
Te2 Te 0.50156(10) 0.52144(8) 0.80781(9) 0.01812(19) Uani 1 1 d .
Te3 Te 0.46468(10) 0.82307(8) 0.48946(8) 0.01745(18) Uani 1 1 d .
Te4 Te 0.49029(10) 0.80979(8) 0.16778(8) 0.01788(19) Uani 1 1 d .
Te5 Te 0.45501(10) 0.48044(8) 0.19661(9) 0.01793(19) Uani 1 1 d .
Te6 Te 0.50093(10) 1.17882(9) 0.51519(9) 0.01800(18) Uani 1 1 d .
Te7 Te 0.47173(10) 1.18742(8) 0.84096(8) 0.01778(19) Uani 1 1 d .
Te8 Te 0.46026(10) 1.16005(7) 0.18367(7) 0.01656(19) Uani 1 1 d .
K1 K 0.2069(4) 0.4741(3) 0.5760(3) 0.0265(5) Uani 1 1 d .
K2 K 0.8281(4) 0.5305(3) 0.3849(4) 0.0413(7) Uani 1 1 d .
K3 K 0.0138(5) 0.6268(4) 0.9095(5) 0.0605(11) Uani 1 1 d .
K4 K 0.9729(4) 1.0755(4) 0.8580(4) 0.0459(8) Uani 1 1 d .
O1 O 0.3812(11) 0.6694(9) 0.8902(10) 0.0235(17) Uani 1 1 d .
O2 O 0.4005(10) 0.9566(8) 0.6902(9) 0.0216(16) Uani 1 1 d .
O3 O 0.3861(10) 0.8655(9) 0.9836(9) 0.0207(16) Uani 1 1 d .
O4 O 0.3078(11) 0.3812(9) 0.9710(9) 0.0250(18) Uani 1 1 d .
O5 O 0.3617(11) 0.6103(9) 0.6760(9) 0.0232(17) Uani 1 1 d .
O6 O 0.5758(12) 0.3830(9) 0.7150(9) 0.0271(19) Uani 1 1 d .
O7 O 0.6669(11) 0.8102(9) 0.5505(9) 0.0226(17) Uani 1 1 d .
O8 O 0.5565(13) 0.7350(9) 0.3637(9) 0.028(2) Uani 1 1 d .
O9 O 0.6046(11) 1.0259(9) 0.2941(9) 0.0231(16) Uani 1 1 d .
O10 O 0.3024(11) 0.9061(9) 0.2358(10) 0.0251(18) Uani 1 1 d .
O11 O 0.3389(12) 0.6304(9) 0.2647(9) 0.0267(18) Uani 1 1 d .
O12 O 0.6524(11) 0.6193(9) 0.0483(10) 0.0265(19) Uani 1 1 d .
O13 O 0.5445(13) 0.4029(10) 0.3623(10) 0.0284(19) Uani 1 1 d .
O14 O 0.6077(11) 0.3255(8) 0.1330(10) 0.0253(18) Uani 1 1 d .
O15 O 0.3128(11) 1.1637(9) 0.4436(10) 0.0239(17) Uani 1 1 d .
O16 O 0.3546(11) 1.2209(9) 0.6695(9) 0.0242(18) Uani 1 1 d .
O17 O 0.6704(11) 1.1137(9) 0.7503(9) 0.0229(17) Uani 1 1 d .
O18 O 0.6083(11) 1.1621(10) -0.0048(9) 0.0258(18) Uani 1 1 d .
O19 O -0.0135(15) 0.3516(14) 0.8788(12) 0.036(3) Uani 0.8 1 d P
O20 O 1.0000(14) 1.2933(11) 0.5357(12) 0.024(2) Uani 0.8 1 d P
O21 O 0.9907(15) 0.6883(11) 0.4790(14) 0.038(4) Uani 0.8 1 d P
O22 O 0.9969(14) 0.7644(14) 0.0934(13) 0.039(3) Uani 0.8 1 d P
O23 O -0.040(2) 0.3507(18) 1.2056(13) 0.058(4) Uani 0.8 1 d P
O24 O 0.0244(14) 0.9070(12) 0.7083(14) 0.039(3) Uani 0.8 1 d P
O25 O 0.9941(17) 1.0170(17) 1.1297(15) 0.048(4) Uani 0.8 1 d P
O26 O 0.9453(17) 1.0336(14) 0.4381(15) 0.045(3) Uani 0.8 1 d P
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.006 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0 0 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Te Te -0.5308 1.6751 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
